General

Property | Value | Condition | Related Standards |
---|---|---|---|

Density | 2.78 g/cm³ Show Material materials with Density of 2.78 g/cm³ | T861 | AA Standards, ASTM B209 |

2.78 g/cm³ Show Material materials with Density of 2.78 g/cm³ | T861 | ||

3.0 g/cm³ Show Material materials with Density of 3.0 g/cm³ | T861 |

Mechanical

Property | Temperature | Value | Condition | Related Standards | Comment |
---|---|---|---|---|---|

Elastic modulus | 73.0 GPa Show Material materials with Elastic modulus of 73.0 GPa | T861 | AA Standards, ASTM B209 | ||

Elongation | -195 °C | 5 % Show Material materials with Elongation of 5 % | T861 | Elongation in 50 mm | |

-80 °C | 5 % Show Material materials with Elongation of 5 % | T861 | Elongation in 50 mm | ||

3.0 % Show Material materials with Elongation of 3.0 % | T861 | AA Standards, ASTM B209 | A50 | ||

3.0 % Show Material materials with Elongation of 3.0 % | T861 | AA Standards, ASTM B209 | A100 | ||

3.5 % Show Material materials with Elongation of 3.5 % | T861 | ||||

4.0 % Show Material materials with Elongation of 4.0 % | T861 | AA Standards, ASTM B209 | A50 | ||

0 °C | 5 % Show Material materials with Elongation of 5 % | T861 | Elongation in 50 mm | ||

24 °C | 5 % Show Material materials with Elongation of 5 % | T861 | Elongation in 50 mm | ||

100 °C | 6 % Show Material materials with Elongation of 6 % | T861 | Elongation in 50 mm | ||

150 °C | 11 % Show Material materials with Elongation of 11 % | T861 | Elongation in 50 mm | ||

205 °C | 28 % Show Material materials with Elongation of 28 % | T861 | Elongation in 50 mm | ||

260 °C | 55 % Show Material materials with Elongation of 55 % | T861 | Elongation in 50 mm | ||

315 °C | 75 % Show Material materials with Elongation of 75 % | T861 | Elongation in 50 mm | ||

370 °C | 100 % Show Material materials with Elongation of 100 % | T861 | Elongation in 50 mm | ||

Plane-Strain Fracture Toughnes | 22.0 - 35.0 MPa·√m Show Material materials with Plane-Strain Fracture Toughnes of 22.0 - 35.0 MPa·√m | Typical for Wrought 2000 Series Aluminium | |||

Poisson's ratio | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | Typical for Wrought 2000 Series Aluminium | |||

Shear modulus | 28.0 GPa Show Material materials with Shear modulus of 28.0 GPa | T861 | |||

Tensile strength | -195 °C | 635 MPa Show Material materials with Tensile strength of 635 MPa | T861 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | |

-80 °C | 558 MPa Show Material materials with Tensile strength of 558 MPa | T861 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

480.0 MPa Show Material materials with Tensile strength of 480.0 MPa | T861 | AA Standards, ASTM B209 | |||

490.0 MPa Show Material materials with Tensile strength of 490.0 MPa | T861 | AA Standards, ASTM B209 | |||

0 °C | 538 MPa Show Material materials with Tensile strength of 538 MPa | T861 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

550.0 MPa Show Material materials with Tensile strength of 550.0 MPa | T861 | ||||

24 °C | 517 MPa Show Material materials with Tensile strength of 517 MPa | T861 | |||

100 °C | 483 MPa Show Material materials with Tensile strength of 483 MPa | T861 | |||

150 °C | 372 MPa Show Material materials with Tensile strength of 372 MPa | T861 | |||

205 °C | 145 MPa Show Material materials with Tensile strength of 145 MPa | T861 | |||

260 °C | 75 MPa Show Material materials with Tensile strength of 75 MPa | T861 | |||

315 °C | 52 MPa Show Material materials with Tensile strength of 52 MPa | T861 | |||

370 °C | 35 MPa Show Material materials with Tensile strength of 35 MPa | T861 | |||

Unlock all property charts | |||||

Yield strength | -195 °C | 586 MPa Show Material materials with Yield strength of 586 MPa | T861 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | |

-80 °C | 531 MPa Show Material materials with Yield strength of 531 MPa | T861 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

425.0 MPa Show Material materials with Yield strength of 425.0 MPa | T861 | AA Standards, ASTM B209 | RP02 | ||

440.0 MPa Show Material materials with Yield strength of 440.0 MPa | T861 | AA Standards, ASTM B209 | RP02 | ||

500.0 MPa Show Material materials with Yield strength of 500.0 MPa | T861 | ||||

0 °C | 510 MPa Show Material materials with Yield strength of 510 MPa | T861 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

24 °C | 490 MPa Show Material materials with Yield strength of 490 MPa | T861 | |||

100 °C | 462 MPa Show Material materials with Yield strength of 462 MPa | T861 | |||

150 °C | 331 MPa Show Material materials with Yield strength of 331 MPa | T861 | |||

205 °C | 117 MPa Show Material materials with Yield strength of 117 MPa | T861 | |||

260 °C | 62 MPa Show Material materials with Yield strength of 62 MPa | T861 | |||

315 °C | 41 MPa Show Material materials with Yield strength of 41 MPa | T861 | |||

370 °C | 28 MPa Show Material materials with Yield strength of 28 MPa | T861 | |||

Unlock all property charts |

Thermal

Property | Temperature | Value | Condition | Related Standards |
---|---|---|---|---|

Coefficient of thermal expansion | 2.3e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.3e-05 1/K | T861 | ||

20 °C | 2.3199999999999998e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.3199999999999998e-05 1/K | T861 | AA Standards, ASTM B209 | |

100 °C | 2.3199999999999998e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.3199999999999998e-05 1/K | T861 | AA Standards, ASTM B209 | |

Unlock all property charts | ||||

Melting point | 500.0 °C Show Material materials with Melting point of 500.0 °C | T861 | ||

505.0 - 635.0 °C Show Material materials with Melting point of 505.0 - 635.0 °C | T861 | AA Standards, ASTM B209 | ||

Specific heat capacity | 870.0 J/(kg·K) Show Material materials with Specific heat capacity of 870.0 J/(kg·K) | T861 | ||

Thermal conductivity | 120.0 W/(m·K) Show Material materials with Thermal conductivity of 120.0 W/(m·K) | T861 | ||

121.0 - 193.0 W/(m·K) Show Material materials with Thermal conductivity of 121.0 - 193.0 W/(m·K) | T861 | AA Standards, ASTM B209 |

Electrical

Property | Value | Condition | Related Standards | Comment |
---|---|---|---|---|

Electrical conductivity | 17000000.0 - 29000000.0 S/m Show Material materials with Electrical conductivity of 17000000.0 - 29000000.0 S/m | T861 | AA Standards, ASTM B209 | |

22000000 S/m Show Material materials with Electrical conductivity of 22000000 S/m | T861 | Typical value | ||

Electrical resistivity | 3.45e-08 - 5.88e-08 Ω·m Show Material materials with Electrical resistivity of 3.45e-08 - 5.88e-08 Ω·m | T861 | AA Standards, ASTM B209 | |

4.5e-08 Ω·m Show Material materials with Electrical resistivity of 4.5e-08 Ω·m | T861 | Typical value | ||

Specific Electrical conductivity | 38.0 % IACS Show Material materials with Specific Electrical conductivity of 38.0 % IACS | T861 | Typical/Derived value |

Chemical properties

Property | Value | Condition | Related Standards |
---|---|---|---|

Aluminium | 90.7 - 94.7 % Show Material materials with Aluminium of 90.7 - 94.7 % | T861 | |

Chromium | 0.1 % Show Material materials with Chromium of 0.1 % | T861 | AA Standards, ASTM B209 |

Copper | 3.8 - 4.9 % Show Material materials with Copper of 3.8 - 4.9 % | T861 | AA Standards, ASTM B209 |

Iron | 0.50 % Show Material materials with Iron of 0.50 % | T861 | AA Standards, ASTM B209 |

0.5 % Show Material materials with Iron of 0.5 % | T861 | ||

Magnesium | 1.2 - 1.8 % Show Material materials with Magnesium of 1.2 - 1.8 % | T861 | AA Standards, ASTM B209 |

Manganese | 0.3 - 0.9 % Show Material materials with Manganese of 0.3 - 0.9 % | T861 | AA Standards, ASTM B209 |

Other | 0.15 % Show Material materials with Other of 0.15 % | T861 | |

Silicon | 0.5 % Show Material materials with Silicon of 0.5 % | T861 | AA Standards, ASTM B209 |

Titanium | 0.15 % Show Material materials with Titanium of 0.15 % | T861 | AA Standards, ASTM B209 |

Zinc | 0.25 % Show Material materials with Zinc of 0.25 % | T861 | AA Standards, ASTM B209 |

Zirconium | 0.2 % Show Material materials with Zirconium of 0.2 % | T861 |

Technological properties

Property | ||
---|---|---|

Brazing | general: no brazing is known or developed | |

Corrosion properties | Stress corrosion cracking: Betriebsschäden in Gebieten mit Zugspannungen quer zur Kornstruktur, Eingeschränkte Schäden an Laborproben (T4,T3, T351, T3510, T3511), d (T6, T861, T81, T851, T8510, T8511), general: sufficient, in principle it should be protected | |

General machinability | General: poor (O), good to acceptable | |

Workability | general (condition): poor(T4, T3, T351, T3510, T3511, T6), not suitable (T361, T861, T81, T851, T8510, T8511) |